A 3D Lattice Model For Fracture Of Concrete : A Multiscale Approach
Abstract
It is quite well known that fracture behavior of concrete is complex and is influenced by several factors. Apart from material properties, geometric parameters influence fracture behavior and one notable phenomenon is size effect. The existence of the size effect in concrete is well known and various attempts to model the behavior is
well documented in literature. However the approach by Bazant to describe the size
effect behavior in concrete has received considerable attention. The major advantage
of developing the size effect law for concrete is the ability to describe the fracture behavior (namely failure strength) of large size structures inaccessible to laboratory testing. The prediction of size effect is done on the basis of laboratory testing of small size geometrically similar structures. In all the models developed earlier heterogeneity of concrete has not been quantitatively simulated. Hence, the complete description considering heterogeneity in concrete is attempted using the lattice model to understand size effect behavior in concrete.
In the present study, a detailed description of the heterogeneity in concrete is at
tempted by 3D lattice structure. Analytical treatment to gain insights to fracture
behavior is difficult and hence a numerical approach capable of handling the het
erogeneous nature of the material is adopted. A parametric study is performed to
understand the influence of various model parameters like mesh size, failure criterion,
softening model. The conventional size effect studies for 2D geometrically similar
structures are performed and a comparison is done with experimentally observed
behavior. The variation of fracture process zone with respect to structure size is
observed as the reason for size effect. The influence of variation in properties of ag
gregate, matrix and interface are studied to explain the deviation in prepeak and
postpeak response. A statistical study is performed to establish the size dependence
of linear regression parameters (Bf ‘t and D0) which are used in Bazant size effect law.
An analytical framework is also proposed to substantiate the above results. Size effect
in concrete is generally attributed to the effect of depth viz. the dimension in the
plane of loads. However although the effect of thickness viz. a dimension in a plane
perpendicular to that of the loads is not considered in concrete. The same is quite
well known in fracture of metals. Therefore the variation in grading of aggregates
along with the influence of thickness on fracture behavior is analysed. To understand
the thickness effect a comparison of 2D and 3D geometrically similar structures is
performed to understand the effect of thickness on fracture parameters.
Heterogeneity is a matter of scale. A material may be homogeneous at a coarser scale while at a finer scale it is heterogeneous. Hence only way to capture the effect of the behavior at micro level on the behavior at meso level particularly in a heterogeneous material like concrete is by a multiscale modelling. The best numerical tool for multiscale model of a heterogeneous material is lattice model. The heterogeneous
nature of concrete is not just due to the presence of aggregates but is evident right
from the granular characteristics of cement. The hydration of cement grain leads to
the development of products with varying mechanical and chemical properties. As
the microcrack initiation and development of thermal cracking is observed at the
micron level, understanding of hydration behavior in concrete can be thought of as
a prerequisite for complete understanding of fracture behavior. The properties of
matrix and interface observed during hydration modelling can also be used as an
input for fracture predictions at upper scale models (eg. mesoscale). This can also be used to study the coupling of scales to understand the multiscale fracture behavior in concrete. A numerical model is hence developed to study the hydration of concrete.
Due to the existence of complex mechanisms governing the hydration behavior in con
crete and the large number of parameters affecting its rate, the hydration of a grain
is assumed to proceed in isolation. A single particle hydration model is developed to
study the hydration of isolated grain. A shrinking core model usually used to describe
the burning of coal is adopted as a base model for analytically describing the hydra
tion behavior. The shrinkage core model in literature is modified to be applicable to
hydration of cement matrix. The effect of particle diameter as well as changing water
concentration is incorporated into the model whereas the influence of reduction in
pore sizes as well as the effect due to embedding of particles and the constraint due
to hydration of neighbouring particles is accounted using correction factor. The effect
of temperature on rate of hydration is considered to be independent of the physical
and chemical aspects of grain. Hence a temperature function developed using Arrhe
nius equation and activation energy is incorporated separately. The porous nature of
reaction products affects the diffusivity leading to the development of tortuous path
for flow of water through the hydrated portion. Knowing the tortuosity it is possible to obtain the diffusivity which in turn can be used as an input to the lattice model.
An algorithm is developed to determine the tortuosity in diffusion of water through
the reaction products. The tortuosity depends on the distribution of pores in the
hydrated system. This requires the use of simulation technique to generate the initial
position of voids. A simulation technique is also required to generate the initial con
figuration of hydrating cement system. In order to generate the initial configurations
of such systems a numerical technique to generate a large scale assembly of particles
is proposed.
In the present work, parameters of Bazant's size effect law Bf’t and D0 are shown
to depend on structure size and heterogeneity. The span to thickness ratio of the structure increases fracture energy and also substantially influences the response of structure. The variation in failure load occurring due to the heterogeneous nature of the material is shown to follow a normal distribution. The fracture behavior of a material is seen to be influenced strongly by the variation in the strength of matrix and interface. The model proposed to describe the hydration process of cement can be used to determine the properties of matrix and interface. The degree of hydration as well as the embedded centre plane area can be adopted as a measure of strength of matrix and interface. The understanding of the hydration process and the wall effect around the aggregate surface can possibly improve our ability to predict the strength of interface. The material strength of the interface is certainly a necessary input to the lattice model. Infact experimental determination of interface strength is a lot more complicated than the present numerical approach. The only weakness of the present numerical approach is the assumption regarding certain empirical constants which of course may be improved further. Understanding of material behavior can be further improved if a molecular dynamics approach is adopted to describe the hydration behavior of cement. The approach via molecular dynamics is suggested as a problem for future research.
Collections
 Civil Engineering (CiE) [232]
Related items
Showing items related by title, author, creator and subject.

Repair and Retrofit Strategies for Structural Concrete against ThermoMechanical Loadings
Guruprasad, Y K (20180129)Reinforced cement concrete (RCC) structures have become an important aspect in most of the buildings in our society around the world. Most of the multistoried reinforced concrete buildings house important institutions such ... 
Concrete Fracture And Size Effect  Experimental And Numerical Studies
Vidya Sagar, R (20101014)Most materials including concrete have preexisting flaws or defects. The fracture energy of concrete is a basic material property needed to understand fracture initiation and propagation in concrete. Whether fracture ...